A New Family of Argyrodite Thioantimonate Lithium Superionic Conductors.
Zhou, Laidong; Assoud, Abdeljalil; Zhang, Qiang; Wu, Xiaohan; Nazar, Linda F.; Journal of the American Chemical Society  (2019) –; doi:10.1021/jacs.9b08357

data_4129176
_publ_section_title
;
 A New Family of Argyrodite Thioantimonate Lithium Superionic Conductors.
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_paper_doi               10.1021/jacs.9b08357
_journal_year                    2019
_chemical_formula_moiety         'Ge0.22 I0.99 Li5.96 S5.01 Sb0.78'
_chemical_formula_sum            'Ge0.22 I0.99 Li5.96 S5.01 Sb0.78'
_chemical_formula_weight         438.46
_space_group_crystal_system      cubic
_space_group_IT_number           216
_space_group_name_Hall           'F -4 2 3'
_space_group_name_H-M_alt        'F -4 3 m'
_audit_creation_method           SHELXL-2016/6
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   10.4128(16)
_cell_length_b                   10.4128(16)
_cell_length_c                   10.4128(16)
_cell_measurement_reflns_used    202
_cell_measurement_temperature    280(2)
_cell_measurement_theta_max      29.796
_cell_measurement_theta_min      3.389
_cell_volume                     1129.0(3)
_computing_cell_refinement       'SMART, 'Bruker APEX II'
_computing_data_collection       'Bruker kappa APEX II'
_computing_data_reduction        'SAINT, 'Bruker APEX II'
_computing_structure_refinement  'SHELXL-2016/6 (Sheldrick, 2016)'
_computing_structure_solution    'SHELXL-2016 (Sheldrick, 2016)'
_diffrn_ambient_temperature      280(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'BRUKER kappa APEX II'
_diffrn_measurement_method       'Omega and phi scan'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0205
_diffrn_reflns_av_unetI/netI     0.0109
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       3
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            2092
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         29.796
_diffrn_reflns_theta_min         3.389
_diffrn_source                   'fine-focus sealed tube'
_exptl_absorpt_coefficient_mu    6.060
_exptl_absorpt_correction_T_max  0.7460
_exptl_absorpt_correction_T_min  0.6660
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
 SADABS 2016/2: Krause, L., Herbst-Irmer, R., Sheldrick G.M. & Stalke D.,
 J. Appl. Cryst. 48 (2015) 3-10
;
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    2.580
_exptl_crystal_description       Plate
_exptl_crystal_F_000             789
_exptl_crystal_size_max          0.080
_exptl_crystal_size_mid          0.050
_exptl_crystal_size_min          0.020
_refine_diff_density_max         0.487
_refine_diff_density_min         -0.145
_refine_diff_density_rms         0.054
_refine_ls_abs_structure_details
;
 Flack x determined using 87 quotients [(I+)-(I-)]/[(I+)+(I-)]
 (Parsons, Flack and Wagner, Acta Cryst. B69 (2013) 249-259).
;
_refine_ls_abs_structure_Flack   0.056(15)
_refine_ls_extinction_coef       0.0007(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2016/6 (Sheldrick 2016)'
_refine_ls_goodness_of_fit_ref   1.167
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     18
_refine_ls_number_reflns         202
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.167
_refine_ls_R_factor_all          0.0090
_refine_ls_R_factor_gt           0.0090
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0172P)^2^+0.0276P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0239
_refine_ls_wR_factor_ref         0.0239
_reflns_Friedel_coverage         0.757
_reflns_Friedel_fraction_full    1.000
_reflns_Friedel_fraction_max     1.000
_reflns_number_gt                202
_reflns_number_total             202
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            Li6.2Ge0.2Sb0.8S5I.cif
_cod_data_source_block           Li6.2Ge0.2Sb0.8S5I
_cod_original_cell_volume        1129.0(5)
_cod_database_code               4129176
_shelx_shelxl_version_number     2016/6
_shelx_estimated_absorpt_t_min   0.643
_shelx_estimated_absorpt_t_max   0.888
_shelx_res_checksum              74006
_shelx_hkl_checksum              28668